Strong and Dynamic CO2 Sorption in a Flexible Porous Framework Possessing Guest Chelating Claws
Pei-Qin Liao; Dong-Dong Zhou; Ai-Xin Zhu; Lu Jiang; Rui-Biao Lin; Jie-Peng Zhang; Xiao-Ming Chen; Journal of the American Chemical Society 134 (2012) 17380–17383; doi:10.1021/ja3073512

data_4118806
_publ_section_title
;
 Strong and Dynamic CO2 Sorption in a Flexible Porous Framework Possessing
 Guest Chelating Claws
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              17380
_journal_page_last               17383
_journal_paper_doi               10.1021/ja3073512
_journal_volume                  134
_journal_year                    2012
_chemical_formula_sum            'C14.07 H16 N12 O0.15 Zn2'
_chemical_formula_weight         486.37
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 95.447(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.6825(13)
_cell_length_b                   12.3388(15)
_cell_length_c                   17.126(2)
_cell_measurement_temperature    195(2)
_cell_volume                     2247.2(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      195(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       '/w scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0301
_diffrn_reflns_av_sigmaI/netI    0.0268
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            17508
_diffrn_reflns_theta_full        26.00
_diffrn_reflns_theta_max         26.00
_diffrn_reflns_theta_min         2.04
_exptl_absorpt_coefficient_mu    2.160
_exptl_absorpt_correction_T_max  0.6720
_exptl_absorpt_correction_T_min  0.5635
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.438
_exptl_crystal_description       block
_exptl_crystal_F_000             982
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.20
_refine_diff_density_max         0.395
_refine_diff_density_min         -0.263
_refine_diff_density_rms         0.068
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.025
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     270
_refine_ls_number_reflns         4373
_refine_ls_number_restraints     5
_refine_ls_restrained_S_all      1.028
_refine_ls_R_factor_all          0.0391
_refine_ls_R_factor_gt           0.0298
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0501P)^2^+0.3804P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0780
_refine_ls_wR_factor_ref         0.0839
_reflns_number_gt                3586
_reflns_number_total             4373
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja3073512_si_002_5.cif
_cod_data_source_block           1_0.07CO2
_cod_original_cell_volume        2247.1(5)
_cod_database_code               4118806